23 January 2023: Lab/In Vitro Research
Comparison of Antibacterial Activity, Cytotoxicity, and Fluoride Release of Glass Ionomer Restorative Dental Cements in DentistryAyse Gunay1ABCDEF*, Sema Celenk1EF, Ozkan Adiguzel 2AE, Suzan Cangul3AEF, Nida Ozcan4BE, Ezgi Eroglu Cakmakoglu5A
Med Sci Monit 2023; 29:e939065
BACKGROUND: This study aimed to compare the antibacterial activity, cytotoxicity, and fluoride release of 4 different glass ionomer cements (GIC).
MATERIAL AND METHODS: A total of 200 samples were prepared: Riva Silver, a silver-reinforced GIC; Equia Forte HT, a glass hybrid GIC; ChemFil Rock, a zinc-added GIC; and Ketac™ Molar Easymix. Using the agar diffusion test for antibacterial activity, 30 samples from each group were analyzed for Streptococcus mutans, Lactobacillus acidophilus, and Actinomyces naeslundii. The areas around the samples where no bacterial growth occurred were digitally measured and recorded. For cytotoxicity analysis, the WST-1 test was performed on 10 samples from each group using the L929 mouse fibroblast cell line. The fluoride release property was evaluated using an ion-selective electrode method on 10 samples from each group.
RESULTS: The group that used Ketac™ Molar Easymix showed the lowest antibacterial activity against S. mutans, L. acidophilus, and A. naeslundii. In all 3 days of cytotoxicity testing, the group that used Riva Silver was found to be the least toxic material, while the group that used ChemFil Rock did not have viable cells after the 1st day. In all 4 materials, fluoride release values gradually increased since the first day, with Ketac™ Molar Easymix having the highest fluoride release.
CONCLUSIONS: Of all the GICs tested, Ketac™ Molar Easymix demonstrated the least antibacterial activity despite having the highest fluoride release, while Riva Silver was found to be the least cytotoxic material.
Keywords: Fluorides, Glass Ionomer Cements
Dental caries is one of the most common chronic diseases observed in people of all ages worldwide . As a result of advancements in dentistry, new minimally invasive techniques and materials have been developed to protect remaining tooth structures and to minimize pulp damage [2–4]. After removing the caries layer using this conservative approach, infected tissues and microorganisms may remain in the dentin cavity [1,5,6]. This situation necessitated the development of materials that increase remineralization and antibacterial activity via their fluoride-releasing properties. GICs, one of the most commonly used materials for this purpose, were introduced to dentistry by Wilson and Kent  in the 1970s.
Conventional GICs (CGICs) are made by combining water-soluble polymeric acids with calcium- or strontium-based alumina-silicate glass powders and adding fluoride . Their advantages include remineralization of dental hard tissues, such as enamel and dentin, as a result of fluoride release; a dentin-like thermal expansion coefficient and modulus of elasticity; chemical bonding to mineralized tooth tissues; good biocompatibility; and an inhibitory effect on the growth of cariogenic bacteria after incomplete caries removal procedures . Despite these advantages, CGICs have some disadvantages, including a long curing time, high sensitivity and brittleness to moisture during the initial curing reaction, microleakage, low wear resistance, and a short working time [10–12]. To minimize these disadvantages and improve mechanical properties, different materials have been added to GIC, and different categories such as resin-modified GICs (RMGICs), metal-reinforced GICs (MRGICs), high-viscosity glass ionomers, and giomers have been developed [9,13].
In minimally invasive approaches, the possibility of microorganisms remaining in the cavity increases the risk of restoration failure due to secondary caries . Secondary and initial caries have similar microbiology. Streptococci, Lactobacilli, and Actinomyces are involved in the early stages of bacterial invasion in caries development. Streptococcus mutans is the primary bacterium responsible for caries formation. Lactobacillus acidophilus is responsible for the progression of caries and the formation of secondary caries. Actinomyces naselundii is associated with root caries and can invade dentinal tubules [15,16]. The use of materials with antibacterial or bactericidal effects, especially in minimally invasive approaches, will provide additional treatment by suppressing residual infection and increasing the life of the restored tooth . Because of their low pH and fluoride-releasing properties, GICs exhibit antibacterial properties immediately after placement in the cavity .
GICs are also known for their ability to remineralize dental hard tissues, such as enamel and dentin, as a result of fluoride release into the oral environment . The release of fluoride from the restorative material and the continuous supply of low levels of fluoride ions in the biofilm–saliva–tooth interaction play important roles in caries prevention .
Although restoration materials help restore tooth health, the products released by these materials can directly or indirectly affect the surrounding tissues as they pass through the dentin canals to the pulp during and after the polymerization process [21,22]. Many of these materials come into contact with or interact with body tissues and fluids; therefore, not only their mechanical and physical properties, but also their biological compatibility should be considered when selecting materials . Biocompatibility is defined as the ability of a material to function in living organisms and induce an appropriate tissue response . The biocompatibility of GICs depends on the components that decompose during the curing process. Given that both components of GICs (glass powder and polyacid liquid) consist of a spectrum of chemical formulas, the risk of these materials causing toxic effects in vivo has been partially evaluated by in vitro tests .
Therefore, this study aimed to compare the antibacterial activities of 4 different GICs against S. mutans, L. acidophilus, and A. naselundii; their cytotoxicity on a mouse fibroblast cell line; and their fluoride release properties.
Material and Methods
PREPARATION OF SAMPLES:
For the analyses, a total of 200 disk-shaped samples (30 for antibacterial activity, 10 for cytotoxicity, and 10 for fluoride release) with a thickness of 2 mm and a diameter of 5 mm were prepared from each material in accordance with the manufacturers’ recommendations, as in the studies of Ranjani et al .
The Riva Silver, Equia Forte HT, and ChemFil Rock GICs in capsule form were mixed in an amalgamator for the time periods specified by the manufacturers. The samples were pressed between a celluloid strip and a glass coverslip and placed in plastic rings using the applicator to prevent air bubble formation, remove excess material, and obtain a flat, smooth surface. After curing at room temperature, the samples removed from the plastic rings were polished with polishing disks.
Ketac™ Molar Easymix was prepared manually by mixing powder and liquid with a spatula. Similarly to other materials, it was pressed between a glass and a celluloid strip and placed in plastic rings. After curing at room temperature, the samples removed from the rings were polished with polishing disks.
EVALUATION OF ANTIBACTERIAL EFFICACY:
The agar diffusion test was performed on 30 samples from each group using standard bacterial isolates of
The agar diffusion test was performed using Mueller-Hinton fastidious (MHF) agar medium, which is recommended for use in antibiotic susceptibility tests of
EVALUATION OF CYTOTOXICITY:
Using the L929 mouse fibroblast cell line, WST-1 analysis was performed on 10 samples from each group. The cells were placed in 24-well culture plates at 1×104 cells/cm2 and incubated for 1 day in an incubator at 37°C and 5% CO2. After subjecting the disk samples to UV sterilization, they were placed in the prepared experimental medium and incubated in a low glucose Dulbecco’s Modified Eagle’s Medium containing 10% fetal bovine serum and 1% penicillin/streptomycin. The control group consisted of L929 cells that had not been treated with any material. After our samples were placed in the experimental environment, WST-1 tests were performed at the end of the 1st, 3rd, and 7th days.
After the samples were removed from the experimental medium on the specified days, WST-1 reagent (WST-1 Cell Proliferation Assay Reagent (Roche)) was added in a 1: 10 ratio. After 2 h of incubation under appropriate conditions, the absorbances were measured at 450 nm using a monochromatic microplate reader (Microplate Reader, VersaMax, Molecular Devices, USA).
EVALUATION OF FLUORIDE RELEASE:
The fluoride releases of 10 samples from each group were evaluated using the ion-selective electrode method.
The ion-selective electrode method was employed for the analyses using the ionometer device (Thermo Orion 720 A+), with a fluoride electrode (Orion 9609 BNWP), a 0.1 MF standard (Orion ionplus-application solution-940906), and a special filling liquid (Orion ionplus-filling solution-900061) placed in the fluoride electrode. The TISAB II solution (Orion ionplus-application solution-940909) was prepared in a 1: 1 ratio and used as an anti-interference buffer. Depending on the concentration range to be studied, 5 calibration standards (0.1, 1, 10, 50, and 100 ppm) were used to calibrate the electrode.
After weighing and recording the weight of each sample with a precision balance, 5 mL of distilled water was added to the sample, and the sample was placed in an oven at 37°C.
On the 1st, 2nd, 3rd, 7th, 14th, 21st, and 28th days, the TISAB II solution was mixed in a 1: 1 ratio with the distilled water taken from the tubes containing the groups, and the reading was taken by immersing the electrode. Before and after each measurement, the electrode tip was washed and lightly dried with distilled water to remove any residual fluoride ions.
SPSS version 22 package program and descriptive statistical methods were used in the statistical evaluation of the data in this study, and a value of
The Kruskal-Wallis test was used for the multiple comparison of the groups, and the Mann-Whitney U test was used for the pairwise comparison of the groups.
The Friedman test was used for multiple comparisons of groups on repetitive days, and the Wilcoxon test was used for pairwise comparisons.
ANTIBACTERIAL EFFICACY FINDINGS:
When we evaluated the antibacterial activity of the 4 different GICs against
When the antibacterial activities against
In the evaluation of antibacterial efficacy against
Table 2 shows inhibition zone mean values and standard deviations in the evaluation of antibacterial activity against S. mutans, L. acidophilus, and A. naeslundii.
When the number of viable cells in the L929 mouse fibroblast cell line was examined using WST-1 analysis of the 4 different GICs used in our study, the majority of cells were observed in the control group on all 3 days, while there were no viable cells in the ChemFil Rock group after the 1st day. The control group was followed by Riva Silver and Equia Forte HT, respectively, while the least number of cells were detected in the group that used Ketac™ Molar Easymix on the 1st day and in the group that used ChemFil Rock on the 3rd and 7th days.
The mean and standard deviations of viable cell numbers as a result of cytotoxicity analysis are shown in Table 3.
FLUORIDE RELEASE FINDINGS:
When the fluoride releases of the 4 GICs were examined, we found that the values increased gradually in each group, starting from the 1st day. While ChemFil Rock yielded the lowest fluoride release values on all measurement days, Ketac™ Molar Easymix yielded the highest fluoride release values. The mean fluoride release values and standard deviations are shown in Table 4.
The dentist’s understanding of the physical, mechanical, and chemical properties of restorative materials used in pediatric dentistry is critical for the longevity of the restorations and patient satisfaction. The closest restorative material to the ideal is the one that has physical properties similar to the dental tissue, bonds well to enamel and dentin, and does not undergo structural changes in the oral environment . Because of their antimicrobial properties, ease of application, and fluoride-releasing properties, GICs are frequently used in dentistry . One of the biggest advantages of GICs is the ability to modify their biological and physical properties by adjusting the powder-to-liquid ratio or changing the chemical formulation to minimize the risk of restoration failure .
The antibacterial activities, cytotoxicity, and fluoride releases of Riva Silver, a silver-reinforced GIC; Equia Forte HT, a glass hybrid GIC; ChemFil Rock, a zinc-added GIC; and Ketac™ Molar Easymix, a CGIC derived from glass ionomer-based materials used in dentistry, were evaluated in this in vitro study.
Because of their fluoride release properties, CGICs promote the formation of fluorapatite on the tooth surface. This substance is less soluble than hydroxyapatite .
Arısu et al  reported that CGICs released the highest amount of fluoride as well as more fluoride compared to MRGICs in their study in which they evaluated fluoride releases of 7 different restorative materials.
In their studies comparing fluoride releases of GICs in different environments, Hattab and Amin  found that CGICs released more fluoride compared to MRGICs. In the study by Bahammam et al  comparing fluoride releases of 4 different GICs, the group using ChemFil Rock showed the least fluoride release on all days.
In our study, the highest fluoride release was observed in the Ketac™ Molar Easymix group, which is the CGIC group, and the least fluoride release was observed in the ChemFil Rock group on all measurement days. This difference between CGICs and MRGICs could be attributed to the faster release of fluoride in the form of NaF and SiF in conventional glass ionomers than fluoride that is bound to silver particles .
Although the amount of fluoride released in the materials indicates the antimicrobial capacity of the material, some researchers reported that the low pH value during the curing reactions of GICs was more effective in terms of the antimicrobial effect than the release of fluoride and did not show any antimicrobial activity after curing was completed [34,35]. Coşgun et al  reported all GICs had low antimicrobial effects. All of the GICs in our study had a low antibacterial effect.
Saxena and Tiwari  evaluated the fluoride-releasing properties and antimicrobial effects of Zirconomer and Fuji IX against S. mutans, Lactobacillus casei, and Candida albicans. In that study, antifungal effects of the GICs used were observed, but it was determined that Zirconomer had a higher antibacterial effect than Fuji IX, a CGIC.
El-Baky and Hussien  showed that Fuji IX inhibited the growth of S. mutans and L. acidophilus, and Shashibhushan et al  demonstrated that Fuji IX inhibited the growth of S. mutans.
In our study, it was found that Ketac™ Molar Easymix inhibited the growth of S. mutans, L. acidophilus, and A. naeslundi, but had the lowest antibacterial effect compared to other GICs.
Many new-generation GICs have been developed and used to improve the mechanical properties of GICs. However, there have been very few comparative studies demonstrating the cytotoxic effects of these materials [24,40]. Therefore, this study aimed to evaluate GICs in terms of cytotoxicity as well as antibacterial and fluoride-releasing properties.
Cell culture, agar diffusion test, filter diffusion test, and dentin barrier test are common cytotoxicity tests . In our study, we used the standard, easy-to-apply, and less time-consuming cell culture method with the L929 (mouse gingival fibroblast) cell line.
In the literature, it is emphasized that low pH during curing and various released components cause cytotoxicity. The fluoride ion released from glass ionomers is the most well-known [41,42].
In their study on the cytotoxicity of CGICs and MRGICs, Selimovic-Dragaš et al  reported that CGICs and silver-reinforced GICs had fewer toxic effects on osteoblast-like cells compared to other materials. In our study, Riva Silver, a silver-reinforced GIC, was found to be the least toxic material. As a result, we believe that the addition of nano-sized silver particles will be a more promising GIC in terms of biosecurity.
Kanjevac et al  investigated the fluoride release of GICs and their cytotoxic effects on human pulp stem cells and concluded that the material that released the most fluoride was the most toxic. In our study, Ketac™ Molar Easymix, which released the most fluoride, was determined to be the most toxic material on the 1st day. On the 3rd and 7th days, it was the most toxic material, followed by ChemFil Rock, which resulted in zero viable cells.
Cell culture data provide insight into the release of undesirable components from this material and possible reactions. These studies should also be supported by in vivo evaluation tests.
This study had some limitations. Only 4 different CCIS were compared with each other. Furthermore, it was tested for a limited period of time, as the analyzes were performed in vitro under laboratory conditions. Given the highly variable conditions of the oral environment, more precise data can be obtained with different types of CIS or other restorative materials and with longer in vitro or in vivo analyzes.
Based on the findings of this in vitro study, all GICs showed varying degrees of antibacterial activity against S. mutans, L. acidophilus, and A. naeslundii but Ketac™ Molar Easymix showed the least. Although the amount of fluoride required to prevent caries has not yet been determined, all materials used in our study released fluoride at different rates. Therefore, long-term fluoride-releasing dental materials should be preferred until the ideal fluoride concentration is determined in patients with high caries risk because the active ingredients in the structure of GICs have a cytotoxic potential and can alter the metabolism of the pulp cell. In our study, Riva Silver was determined to be the least cytotoxic material. This cytotoxic effect should be considered when using the GICs employed in our study.
1. Sagmak S, Bahsi E, Ozcan N, Satici O, Comparative evaluation of antimicrobial efficacy and fluoride release of seven different glass-ionomer-based restorative materials: Oral Health Prev Dent, 2020; 18; 521-28
2. Bjørndal L, Larsen T, Changes in the cultivable flora in deep carious lesions following a stepwise excavation procedure: Caries Res, 2000; 34; 502-8
3. Maltz M, Oliveira EF, Fontanella V, Carminatti G, Deep caries lesions after incomplete dentine caries removal: 40-month follow-up study: Caries Res, 2007; 41; 493-96
4. Oliveira EF, Carminatti G, Fontanella V, Maltz M, The monitoring of deep caries lesions after incomplete dentine caries removal: Results after 14–18 months: Clin Oral Invest, 2006; 10; 134-39
5. Duque C, Negrini TC, Sacomo NT, Clinical and microbiological performance of resin-modified glass-ionomer liners after incomplete dentine caries removal: Clin Oral Invest, 2009; 13; 465-71
6. Weerheijm KL, Kreulen CM, de Soet JJ, Groen H, van Amerongen W, Bacterial counts in carious dentine under restorations: 2-year in vivo effects: Caries Res, 1999; 33; 130-34
7. Wilson AD, Kent BE, Glass-ionomer cement, a new translucent dental filling material: J Appl Chem Biotechnol, 1971; 21; 313
8. Elmacı I, Tunçdemir MT, Restoratif diş hekimliğinde cam iyonomer simanlar ve yeni gelişmeler: NEU Dent J, 2020; 2; 69-75 [in Turkish]
9. Ersahan S, Oktay EA, Sabuncuoglu FA, Evaluation of the cytotoxicity of contemporary glass-ionomer cements on mouse fibroblasts and human dental pulp cells: Eur Arch Paediatr Dent, 2020; 21; 321-28
10. Mickenautsch S, Mount G, Yengopal V, Therapeutic efect of glass ionomers: An overview of evidence: Austr Dent J, 2011; 56; 10-15
11. Chen S, Mestres G, Lan W, Cytotoxicity of modified glass ionomer cement on odontoblast cells: J Mater Sci Mater Med, 2016; 27; 1-6
12. Sidhu SK, Glass-ionomer cement restorative materials: A sticky subject?: Aust Dent J, 2011; 56; 23-30
13. Tamilselvam S, Divyanand MJ, Neelakantan P, Biocompatibility of a conventional glass ionomer, ceramic reinforced glass ionomer, giomer and resin composite to fibroblasts: In vitro study: J Clin Pediatr Dent, 2013; 37; 403-6
14. Sherief DI, Fathi MS, Abou El Fadl RK, Antimicrobial properties, compressive strength and fluoride release capacity of essential oil-modified glass ionomer cements – an in vitro study: Clin Oral Investig, 2021; 25; 1879-88
15. Mei ML, Li QL, Chu CH, Antibacterial effects of silver diamine fluoride on multi-species cariogenic biofilm on caries: Ann Clin Microbiol Antimicrob, 2013; 12; 4
16. Naik RG, Dodamani AS, Khairnar MR, Comparative assessment of antibacterial activity of different glass ionomer cements on cariogenic bacteria: Restor Sent Endod, 2016; 41; 278-82
17. Farrugia C, Camilleri J, Antimicrobial properties of conventional restorative filling materials and advances in antimicrobial properties of composite resins and glass ionomer cements – a literature review: Dent Mater, 2015; 31; 89-99
18. Tüzüner T, Dimkov A, Nicholson JW, Nicholson. The effect of antimicrobial additives on the properties of dental glass-ionomer cements: A review: Acta Biomater Odontol Scand, 2019; 5; 9-21
19. Hosida TY, Delbem ACB, Morais LA, Ion release, antimicrobial and physio-mechanical properties of glass ionomer cement containing micro or nanosized hexametaphosphate, and their effect on enamel demineralization: Clin Oral Investig, 2019; 23; 2345-54
20. Peroš K, Šutej I, The cariostatic mechanisms of fluoride: Acta Med Acad, 2013; 42; 179-88
21. Kölüş T, Ülker HE, İki farklı rezin modifiye cam iyonomer simanın bölgesel toksisitesinin değerlendirilmesi: Selcuk Dental Journal, 2020; 7(3); 413-21 [in Turkish]
22. Murray PE, García Godoy C, García Godoy F, How is the biocompatibilty of dental biomaterials evaluated?: Med Oral Patol Oral Cir Bucal, 2007; 12; 258-66
23. de Souza Costa CA, Hebling J, Garcia-Godoy F, Hanks CT, In vitro cytotoxicity of five glass-ionomer cements: Biomaterials, 2003; 24(21); 3853-58
24. Marczuk-Kolada G, Łuczaj-Cepowicz E, Pawińska M, Hołownia A, Evaluation of the cytotoxicity of selected conventional glass ionomer cements on human gingival fibroblasts: Adv Clin Exp Med, 2017; 26(7); 1041-45
25. Selimović-Dragaš M, Huseinbegović A, Kobašlija S, Hatibović-Kofman Š, A comparison of the in vitro cytotoxicity of conventional and resin modified glass ionomer cements: Bosn J Basic Med Sci, 2012; 12; 273-78
26. Ranjani MS, Kavitha M, Venkatesh S, Comparative evaluation of osteogenic potential of conventional glass-ionomer cement with chitosan-modified glass-ionomer and bioactive glass-modified glass-ionomer cement an ın vitro study: Contemp Clin Dent, 2021; 12(1); 32-36
27. Erdem AP, Gençay K, Kanıta dayalı diş hekimliği kapsamında cam iyonomer simanların önerilen klinik kullanım alanları: Atatürk Üniv Diş Hek Fak Derg, 2013; 23; 123-30 [in Turkish]
28. Khoroushi M, Keshani F, A review of glass-ionomers: From conventional glass-ionomer to bioactive glass-ionomer: Dent Res J (Isfahan), 2013; 10(4); 411-20
29. Baig MS, Fleming GJ, Conventional glass-ionomer materials: A review of the developments in glass powder, polyacid liquid and the strategies of reinforcement: J Dent, 2015; 43(8); 897-912
30. Hasan AM, Sidhu SK, Nicholson JW, Fluoride release and uptake in enhanced bioactivity glass ionomer cement (“glass carbomer™”) compared with conventional and resin-modified glass ionomer cements: J Appl Oral Sci, 2019; 27; e20180230
31. Arısu HD, Bala O, Üçtaşlı MB, Kalaycı S, Cam iyonomer siman ve poliasit modifiye kompozit rezinlerin florid salma özellikleri: Gazi Üniv Diş Hek Fak Derg, 2007; 24; 157-61 [in Turkish]
32. Hattab FN, Amin WM, Fluoride release from glass ionomer restorative materials and the effect of surface coating: Biomaterials, 2001; 22; 1449-58
33. Bahamman S, Nathanson D, Fan Y, Assessing the release of the fluoride ion in four restorative glass ionomer cements: Fluoride, 2020; 53(4); 611-20
34. Yesilyurt C, Er K, Tasdemir T, Antibacterial activity and physical properties of glass-ionomer cements containing antibiotics: Oper Dent, 2009; 34; 18-23
35. Türkün LS, Türkün M, Ertugrul F, Ates M, Brugger S, Long-term antibacterial effects and physical properties of a chlorhexidine-containing glass ionomer cement: J Esthet Restor Dent, 2008; 20; 29-44
36. Cosgun A, Bolgul B, Duran N, In vitro investigation of antimicrobial effects, nanohardness, and cytotoxicity of different glass ionomer restorative materials in dentistry: Niger J ClinPract, 2019; 22; 422-31
37. Saxena S, Tiwari S, Energy dispersive X ray microanalysis, fluoride release, and antimicrobial properties of glass ionomer cements indicated for atraumatic restorative treatment: J Int Soc Prev Community Dent, 2016; 6; 366-72
38. Abd El-Baky RM, Hussien SM, Comparative antimicrobial activity and durability of different glass ionomer restorative materials with and without chlorohexidine: J Adv Biotechnol Bioeng, 2013; 1; 14-21
39. Shashibhushan KK, Basappa N, Subba Reddy VV, Comparison of antibacterial activity of three fluorides- and zinc-releasing commercial glass ionomer cements on strains of mutans streptococci: An in vitro study: J Indian Soc Pedod Prev Dent, 2008; 26; 56-61
40. Ahmed HMA, Omar NS, Luddin N, Cytotoxicity evaluation of a new fast set highly viscous conventional glass ionomer cement with L929 fibroblast cell line: J Conserv Dent, 2011; 14; 406-8
41. Schmid-Schwap M, Franz A, König F, Cytotoxicity of four categories of dental cements: Dent Mater, 2009; 25; 360-68
42. Hatton PV, Hurrell-Gillingham K, Brook IM, Biocompatibility of glass-ionomer bone cements: J Dent, 2006; 34; 598-601
43. Kanjevac T, Milovanovic M, Volarevic V, Cytotoxic effects of glass ionomer cements on human dental pulp stem cells correlate with fluoride release: Med Chem, 2012; 8; 40-45
01 Jun 2023 : Clinical ResearchRoot Canal Numbers and Configurations in 1080 Permanent Canine Teeth in 270 Saudi Subjects Using Cone-Beam ...
Med Sci Monit In Press; DOI: 10.12659/MSM.940472
01 Jun 2023 : Clinical ResearchInternal Orifice Alloy Closure: A New Procedure for Treatment of Perianal Fistulizing Crohn’s Disease
Med Sci Monit In Press; DOI: 10.12659/MSM.940873
01 Jun 2023 : Clinical ResearchEffectiveness of Needle Aspiration versus Surgical Excision for Symptomatic Synovial Cysts of the Hip: A Si...
Med Sci Monit In Press; DOI: 10.12659/MSM.940187
01 Jun 2023 : Clinical ResearchInfluence of Insulin Resistance on Diabetes Nephropathy
Med Sci Monit In Press; DOI: 10.12659/MSM.939482
Most Viewed Current Articles
13 Nov 2021 : Clinical ResearchAcceptance of COVID-19 Vaccination and Its Associated Factors Among Cancer Patients Attending the Oncology ...
Med Sci Monit 2021; 27:e932788
30 Dec 2021 : Clinical ResearchRetrospective Study of Outcomes and Hospitalization Rates of Patients in Italy with a Confirmed Diagnosis o...
Med Sci Monit 2021; 27:e935379
08 Mar 2022 : Review articleA Review of the Potential Roles of Antioxidant and Anti-Inflammatory Pharmacological Approaches for the Man...
Med Sci Monit 2022; 28:e936292
01 Jan 2022 : EditorialEditorial: Current Status of Oral Antiviral Drug Treatments for SARS-CoV-2 Infection in Non-Hospitalized Pa...
Med Sci Monit 2022; 28:e935952